Spin crossover behaviour in one-dimensional Fe(II) compounds based on the [M(CN)4](2-) (M = Pd, Pt) units.
Zhang, Shao-Liang; Zhao, Xin-Hua; Wang, Yuan-Min; Shao, Dong; Wang, Xin-Yi; Dalton transactions (Cambridge, England : 2003) 44 (2015) 9682–9690; doi:10.1039/c5dt00836k

data_7034992
_publ_section_title
;
 Spin crossover behaviour in one-dimensional Fe(II) compounds based on the
 [M(CN)4](2-) (M = Pd, Pt) units.
;
_journal_issue                   20
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              9682
_journal_page_last               9690
_journal_paper_doi               10.1039/c5dt00836k
_journal_volume                  44
_journal_year                    2015
_chemical_formula_moiety         'C16 H16 Fe N8 Pt'
_chemical_formula_sum            'C16 H16 Fe N8 Pt'
_chemical_formula_weight         571.31
_chemical_melting_point          ?
_chemical_name_common            Fe-pic-Pt(CN)4-HS
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 126.470(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.2838(11)
_cell_length_b                   15.6772(16)
_cell_length_c                   16.0125(12)
_cell_measurement_reflns_used    5232
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      31.10
_cell_measurement_theta_min      2.37
_cell_volume                     2076.0(4)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    Diamond
_computing_publication_material  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker ApexDuo'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0214
_diffrn_reflns_av_unetI/netI     0.0237
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            13175
_diffrn_reflns_theta_full        26.73
_diffrn_reflns_theta_max         26.73
_diffrn_reflns_theta_min         2.05
_exptl_absorpt_coefficient_mu    7.445
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.4140
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS v.2.10 (Bruker,2008) was used for absorption correction.
R(int) was 0.0446 before and 0.0214 after correction.
The Ratio of minimum to maximum transmission is 0.5552.
The l/2 correction factor is 0.0015.
;
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    1.828
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1088
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.16
_refine_diff_density_max         1.065
_refine_diff_density_min         -0.897
_refine_diff_density_rms         0.101
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.036
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     284
_refine_ls_number_reflns         4405
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.036
_refine_ls_R_factor_all          0.0339
_refine_ls_R_factor_gt           0.0247
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0373P)^2^+2.7380P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0757
_refine_ls_wR_factor_ref         0.0817
_reflns_number_gt                3434
_reflns_number_total             4405
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5dt00836k2.cif
_cod_data_source_block           Fe-pic-Pt(CN)4-HS
_cod_depositor_comments
;
The following automatic conversions were performed:

'_chemical_melting_point' value 'not measured' was changed to '?' -
the value is undefined or not given.

Automatic conversion script
Id: cif_fix_values 3271 2015-04-21 07:52:19Z andrius 

 Adding full bibliography for 7034989--7034996.cif.
;
_cod_original_cell_volume        2076.0(3)
_cod_original_sg_symbol_H-M      P2(1)/c
_cod_database_code               7034992